Owned by the authors, published by EDP Sciences, 2015
Research of dynamic properties of alloys of AMg6BM and AMg6M in
shock-wave experiment on a gas gun
S.S. Mokrushin, E.I. Karnaukhov, S.N. Malugina, D.N. Kazakov, O.E. Kozelkov, and A.V. Pavlenkoa
FSUE Zababakhin RFNC-VNIITF, 456770, Snezhinsk
Abstract. Spall strength and elastoplastic parameters of aluminum alloys AMg6BM and AMg6M were studied in shock wave experiments with light gas guns LGG-1200 and LGG-2500 and results of these experiments are provided. Strength wave profiles were registered simultaneously by VISAR and interferometer PDV. Consideration was given to dependences of spall strength and strength parameters of aluminum alloys AMg6BM and AMg6M on the amplitude of the shock-wave loading in the range of 1.1 to 14.2 GPa and on deformation rate in the range of 0.2 to 3.6·105s−1. Threshold damage levels for alloys AMg6M and
AMg6BM are determined. It was shown that alloy AMg6BM softens under the pressure more than 5 GPa.
Aluminum alloys of the system Al-Mg (magnalia) combine good strength and high plasticity, have high processibility, are well distorted, have satisfactory corro-sion resistance and good fusability. This determines wide application of these alloys in atomic industry, building industry, aviation, rocket building, in constructions subjected to high thermal and force loadings [1,2]. Russian industry proves semifinished alloyAMg6 in the form of sheets, rods, foils, profiles in thermally unprocessed (AMg6), annealed (AMg6M), with technological cladding of sheets (AMg6BM) or without cladding (AMg6M), in cold-worked (AMg6N) and other states of products. Prediction of the results of pulse impact on such structures is an important practical task. In order to solve this task, it is necessary to know dynamic, kinematic and thermophysical properties of such structures [3,4].
Authors of [5–8] got the first experimental data on strength characteristics of alloys AMg6 and AMg6M in the conditions of explosive impact with microsecond duration of loading pulse at deformation rate in the range of 103 to 106s−1 and the temperature in the range of (−13◦C) to +550◦C. However, specialists performing experiments described in [5–8] used various approaches in measuring techniques. In activities [5–7], the fact of presence or absence of a spall was determined by visual examination or metallographic study of the samples that were recovered after experiments, and determination of the values of destructing stresses was made by assessment methods (using acoustic spall theory or EOS of the sample material and impactor). In , for determination of values of destructing stresses, the authors used profiles of rate W (t) that were obtained with the help of capacitive pick-up of pressure. The use of various measuring methods led to sufficient disagreement of experimental results [5–8],
especially while determining threshold levels of samples destruction (∼by a factor of 2).
While experimental equipment was developed in [9, 10], the study of dynamic properties of AMg6M was continued. Registration of profiles of free surface of samples was made with the help of laser-interferometric measuring methods. As the result, new experimental data on dynamic properties of AMg6M at deformation rate in the range of 103 to 106s−1, pressure from 2 to 56 GPa, temperature from +20 to +600◦C were obtained at qualitatively new level. Dynamic properties of AMg6 at deformation rate 190 – 1450 s−1using split Hopkinson bar were studied by the authors of .
However, high deformation rates and loading levels realized under using explosive devices did not permit to study in details the regions with transition from elastic to plastic deformation. That is why it is more expedient to use such experimental data for building wide-range mathematical models [3,4]. The development of up-to-date models of elasto-visco-plastic deformation of structural materials [12,13] that are used at our Institute is performed by comparison of experimental profiles of free surface velocity for materials under study and calculation data. In order to accurately determine numerical codes , select parameters of material model , one needs detailed investigation into dynamic properties of materials with smooth change of deformation rate and amplitude of shock-wave impact. It is necessary to note that comparison of strength properties of AMg6 samples fabricated out of rod and sheet material was performed only in [5,7] in the field of pressures up to 3 GPa while investigating threshold levels of the sample destruction. That is why the question about the influence of technological processing of materials on dynamic properties of AMg6M and AMg6BM samples remains unclear. Authors of [14,15] paid much attention to this topic.
This presentation gives the results of investigation into dynamic properties of aluminum alloy AMg6M and alloy AMg6BM. Contrary to [6,8–10], in order to clarify the
Figure 1. Scheme of loading and measuring methods.
influence of technological processing on the properties of materials under study, the samples were fabricated out of AMg6M KR40 rod (GOST 21488-97) and AMg6BM 5 sheet (GOST 21631-76).
Investigation was performed on two one-stage light gas guns  according to method of impact with simultaneous use of two-channel interferometer VISAR  and interferometer PDV . The pressure in the samples was varied in the range from 1.1 to 14.2 GPa, deformation rate – in the range from 0.2 to 3.6·105s−1.
Experimental data were obtained in the form of profiles of free surface velocity W (t) for each type of samples of AMg6M and AMg6BM. Experimental data were processed and analyzed, the values of spall strength, dynamic yield limit, elastic limit and shear stress were determined. Threshold values of pressure were also determined, under which, spall destruction begins. For each material, dependences of spall strength on amplitude of loading pulse and deformation rate were built. Experimental profiles were used for determination of parameters of Johnson-Cook material model with Mie-Gruneisen.
2. Experimental equipment
Experimental studies of dynamic properties of aluminum alloy samplesAMg6M and AMg6BM were performed on light gas guns (LGG) with caliber 44 mm. Collision velocity was varied in the range of 0.2 to 2 km/s. Figure1 shows the scheme of alloys samples loading and applied measuring methods.
In all experiments, evolution of shock waves in the samples of AMg6M and AMg6BM was studied. In experiments with aluminum alloy AMg6M, the technology of forming high deformation rates was probed at the cost of using impactors out of tantalic foils. Data on experiment set-up are given in Tables 1 and 2.
The velocity of impactor collision with the sample V0 was determined with the help of electro-contact gauges. In addition, they determined the value of a slope, which characterized disalignment (distortionϕ) of collided surfaces of impactor with the sample. Registration of profiles of stress waves was made simultaneously with the help of two-channel laser-interferometric complex VISAR and interferometer PDV. That permitted to make registration of velocity profiles W (t) with an error less than 9 m/s and time resolution at least 2,2 ns.
We are investigated aluminum alloy made out of a sheet AMg6BM 5 (GOST 21631-76) and rod AMg6M KR40 (GOST 21488-97). Metallographic analysis of the check test piece for alloy AMg6M confirmed the presence
Table 1. Data on experiment set-up with the samples out of
aluminum alloy AMg6BM.
Impactor Sample No AMg6M, V0, ϕ, AMg6BM,
mm m/s mrad mm 025 2.02 599 3.00 3.80 026 1.99 869 2.34 3.80 027 2.01 383 1.42 3.80 028 2.01 227 1.54 3.80 029 2.02 164 0.92 3.81 031 2.00 231 0.78 3.80 032 2.01 223 0.25 3.80 036 2.01 158 0.93 3.80 040 2.04 196 0.30 3.81 220 2.06 1688 10.37 3.81 221 2.02 1449 3.69 3.80
Table 2. Data on experiment set-up with the samples out of
aluminum alloy AMg6M.
Impactor Thickness, V0, ϕ, Sample
No material mm m/s mrad AMg6M, mm 044 AMg6M 2.05 855 1.10 3.99 047 AMg6M 2.00 570 0.75 3.99 048 AMg6M 2.04 369 0.25 4.00 050 AMg6M 2.04 232 0.9 3.99 051 AMg6M 1.98 184 1.32 4.00 053 AMg6M 2.01 212 0.94 4.00 054 Tantalum 0.05 568 1.02 4.00 058 Tantalum 0.05 569 1.92 2.03 229 AMg6M 2.02 1252 1.74 4.02 230 AMg6M 2.03 1844 21.4 4.01 231 Tantalum 0.05 1285 11.0 3.99 234 AMg6M 2.04 2000 – 4.00
Table 3. Chemical composition (in %) of alloy AMg6 (GOST
Al Cu Mg Mn Fe
Base <0.1 5.8–6.8 0.5–0.8 <0.4 Si Zn Ti Be Sum of impurities
<0.4 <0.2 <0.10 <0.005 0.1
Table 4. Chemical composition (in %) of cladding layer (GOST
components Impurities, not more than
Al Fe Sr Cu Mn Sum of
Not less 0.30 0.30 0.02 0.025 permissible than 99.30 Zn Ti Mg Other impurities
0.1 0.15 0.05 impurities 0.02 0.70
of alternating big and small grains, and this fact speaks about thermal processing of material. The size of big grains was (76±23)µm, the size of small ones was (15±4)µm. Table 3 shows the chemical composition of alloy AMg6 (GOST 4784-97).
For cladding of sheets, aluminum with chemical composition shown in the Table4is used.
Table 5. Data on the sound velocity in the samples of
alloysAMg6BM and AMg6M.
Material Cl, m/s Cs, m/s C0, m/s
AMg6BM 6460±15 3167±15 5325 AMg6M 6487±15 3197±15 5334
Figure 2. Profiles of free surface velocity in experiments with
density of samples was calculated. The mass of samples was measured with the help of laboratory electronic scales of HR-I series. The diameter and thickness of all samples was measured by a linear displacement transducer with 10µm absolute accuracy. Measurement of each parameter of the sample was made 10 times. The error of measurements was calculated at reliability P=0.95 (Student’s coefficient tα=2.26, at n=10 measurements of a parameter). Measured density of AMg6M samples was ρ=2.62±0.02 g/cm3, and density of AMg6BM samples wasρ =2.62±0.01 g/cm3.
Preliminary, the sound velocity was determined for the samples of AMg6M and AMg6BM. The velocity of longitudinal wave Cl was determined using ultra
sound thickness gauge T-MIKE E, and measurement of transverse wave velocity Cs – using electromagnetic
acoustic method of excitation and pick-up of ultra sound waves. Table 5 shows the data about sound velocity for mentioned samples.
3. The results of studies
The studies of dynamic properties of alloys AMg6B and AMg6M we are made in two series of experiments (Tables1 and2). The presence of spall destruction was fixed according to appearance so called “spall” signals on amplitude-time dependences of free surface velocity W (t) that speak about relaxation of stress waves under destruction in the samples . The amplitude of shock-wave impact was varied in the range of 1.1 to 14.2 GPa (the range of collision velocity was from 0.15 to 2 km/s), deformation rate was from 0.2 to 3.6·105s−1. Figures2 and 3 show the profiles of free surface velocity W (t) obtained in experiments with samples of AMg6BM and AMg6M, respectively.
Figure 3. Free surface velocity profiles in the experiments with
AMg6M alloy samples.
Figure 4. Velocity profiles W (t) in the experiments with
AMg6BM (a) and AMg6M (b) alloy samples.
Threshold damage levels for tested materials were determined during the work. Figure 4(a,b) contains velocity profiles W (t) for AMg6BM and AMg6M alloys.
In Fig. 4(a,b) we can see, that spall pulse can be registered at a collision velocity higher than 196 m/s (for AMg6BM alloy) and 212 m/s (AMg6M alloy). No damages, able to form spall signal, are caused at a collision velocity lower than 164 m/s (for AMg6BM alloy) and 184 m/s (for AMg6M alloy).
Figure 5. W (t) velocity profiles in the experiments with AMg6M
Figure 6. Spall strength of AMg6M and AMg6BM alloys
samples depending on the amplitude of shock compression.
rate range using loading technology of AMg6M alloy sample loading with tantalum foils 50µm thick. In Fig.5, we can see free surface velocity profiles for AMg6M alloy; these profiles are formed in the samples with these strikers. Technology used to form load pulses in the samples allowed to extend the deformation rate range to 3.6· 105s−1. But spall signal under conditions shown in Table2 was registered only in one experiment 48. AMg6M alloy spall strength for this experiment wasσsp=1.33 GPa.
Large number of experiments allowed to determine statistical straggling for the Hugoniot limit values (σhel), shear stress values (τT) and dynamic yield limit values (στ). These parameters for AMg6M alloy were the follow-ing:σhel=0.42±0.03 GPa,τT =0.10±0.01 GPa,στ = 0.20±0.01 GPa. For AMg6BM alloy: σhel=0.40± 0.02 GPa,τT=0.10±0.01 GPa,στ =0.19±0.01 GPa.
In Figs. 6 and 7, we can see dependencies of spall strength for alloys AMg6M and AMg6BM on shock compression amplitude and on deformation rate, respectively.
In Figs. 6–7, we can see that spall strength of aluminum alloy AMg6M monotonously increases with pressure increase in the sample in the range from 1.4 to 14.2 GPa. Nevertheless, changes in spall strength of AMg6BM aluminum alloy bear clear-cut softening character at shock compression amplitudes higher than 5 GPa, and deformation rate higher than 0.5·105s−1. It is hardly probable that cladding of AMg6BM sheets will change the material strength. The difference between
Figure 7. Spall strength of AMg6M and AMg6BM aluminum
alloys samples depending on deformation rate.
Figure 8. Spall strength of AMg6M and AMg6BM aluminum
alloys samples depending on deformation rate.
AMg6M and AMg6BM lies only in the technologies of mechanical processing, which influences the material texture. All samples of AMg6BM alloy were manufactured out of the same sheet, thus intercrystalline corrosion of the material couldn’t cause noticed alloy softening. It seems that material rolling changed its interior structure, which led to softening of the material AMg6BM.
Comparison of the experimental results, obtained using LGG, with the results, published in literature [8–10] (see Fig. 8), has shown that spall strength of bar material AMg6M is significantly higher than the one of the sheet material AMg6M. The same destruction character was observed in earlier works [5,7] while studying threshold values for destruction of AMg6 alloy samples, made of bar and of sheet. But some new previously unnoticed peculiar features in material response to shock-wave loading were found in sheet material AMg6M and AMg6BM. These features concerned deformation rate 104–105s−1.
made of bars of AMg6M KR40 (GOST 21488-97) and sheet AMg6BM 5 (GOST 21631-76).
Experimental data is given in the form of sample free surface velocity profiles. Experimental results are analysed. Dependencies of spall strength on amplitude of shock-wave action σ(P) and deformation rate σ( ˙τ) are constructed.
The work results reveal that:
– the dependencies σ(P) and σ( ˙τ) for both sample materials monotonously increase up to the pressure of 5 GPa and ˙τ =0.5·105s−1;
– when pressure is higher than 5 GPa and deformation rate is more than 0.5·105s−1, softening of AMg6BM alloy takes place;
– threshold values of spall strength wereσ =1.4 GPa for AMg6BM alloy, and σ =1.5 GPa for AMg6M alloy, respectively.
Experimental velocity W (t) profiles obtained were used to determine the parameters of Jonson-Cook model of the material with Mie-Gr¨uneisen equation of state. Experimental data satisfactorily agreed with numerical data.
 Physical material science, 6. Construction materials of nuclear power industry/Executive editor B. Kalin (2012)
 V. Belezkii, G. Krivov, Reference book: Aluminum alloys (composition, properties, technology, applica-tion) (2005)
 G. Kangel, V. Fortov, S. Razorenov, A. Utkin, Shock-wave phenomena in condensed media (1996)
 E. Avrorin, B. Vodolaga, V. Simonenko, V. Fortov, Progress in Physical Science Magazine, 163, 5, 1–34 (1993)
 B. Tarasov, Strength problems, 3, 121–122 (1974)  Yu. Batkov, S. Novikov, V. Sinitsin et al., PMTF, 3,
 V. Golubev, S. Novikov, Yu. Sobolev, N. Yukina, Strength problems, 2, 53–59 (1983)
 G. Kanel, S. Razorenov, V. Fortov, PMTF, 5, 60–64 (1984)
 G. Kanel, S. Razorenov, V. Fortov, DAS USSR, 294, 2, 350–352 (1987)
 S. Razorenov, G. Kanel, V. Fortov, FMM, 95, 1, 91– 96 (2003)
 B. Glushak, O. Ignatova, V. Pushkov et al., PMTF, 41, 6, 139–142 (2000)
 A. Petrovtsev, G. Kovalenko, G. Zadorozhniy, Zababakhin Scientific Talks: Sourcebook of VII In-ternational conference – Snezhinsk; RFNC-VNIITV publishers (2003)
 Johnson G.R., Cook W.H., Proc. Of 7t h symposium
of ballistics, Den Hague, Niderlands (1983)
 V. Chuveldeev, M. Gryaznov, V. Kopilov, A. Sisoev, Vestnik Nizhegorodskogo Universiteta, 4, 35–42 (2008)
 B. Kolachev, V. Elagin, V. Livanov. Physical metallurgy and thermal treatment of nonferrous metals and alloys (2005)
 A. Pavlenko, S. Balabin, O. Kozelkov, D. Kazakov, Instr. and Exp. Tech., 4, 122–124 (2013)
 A. Pavlenko, S. Malyugina, V. Pereshitov, I. Lisitsina, Instr. and Exp. Tech., 2, 127–129 (2013)